#------------------------------------------------------------------------------
#$Date: 2016-03-23 16:41:03 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179389 $
#$URL: svn://www.crystallography.net/cod/cif/4/32/86/4328643.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4328643
loop_
_publ_author_name
'Ping Chai'
'John D. Corbett'
_publ_section_title
;
 Gold Derivatives of Eight Rare-Earth-Metal-Rich Tellurides: Monoclinic
 R7Au2Te2 and Orthorhombic R6AuTe2 Types
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              3548
_journal_page_last               3556
_journal_paper_doi               10.1021/ic202342v
_journal_volume                  51
_journal_year                    2012
_chemical_formula_sum            'Au2 Ho7 Te2'
_chemical_formula_weight         1803.64
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 104.427(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   17.978(3)
_cell_length_b                   4.0073(6)
_cell_length_c                   16.997(3)
_cell_measurement_reflns_used    1154
_cell_measurement_temperature    273(2)
_cell_measurement_theta_max      27.06
_cell_measurement_theta_min      2.91
_cell_volume                     1185.9(3)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      273(2)
_diffrn_measured_fraction_theta_full 0.956
_diffrn_measured_fraction_theta_max 0.956
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0515
_diffrn_reflns_av_sigmaI/netI    0.0552
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            5219
_diffrn_reflns_theta_full        28.23
_diffrn_reflns_theta_max         28.23
_diffrn_reflns_theta_min         1.24
_exptl_absorpt_coefficient_mu    75.495
_exptl_absorpt_correction_T_max  0.0336
_exptl_absorpt_correction_T_min  0.0206
_exptl_absorpt_correction_type   none
_exptl_crystal_density_diffrn    10.102
_exptl_crystal_density_meas      0
_exptl_crystal_F_000             2924
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.14
_refine_diff_density_max         3.118
_refine_diff_density_min         -2.937
_refine_diff_density_rms         0.656
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.027
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     69
_refine_ls_number_reflns         1600
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.027
_refine_ls_R_factor_all          0.0514
_refine_ls_R_factor_gt           0.0368
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0324P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0719
_refine_ls_wR_factor_ref         0.0775
_reflns_number_gt                1305
_reflns_number_total             1600
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic202342v_si_002.cif
_cod_data_source_block           722x
_cod_database_code               4328643
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Au1 Au 0.17125(5) 0.0000 0.11128(6) 0.0152(2) Uani 1 2 d S
Au2 Au 0.38078(5) 0.0000 0.60065(6) 0.0160(2) Uani 1 2 d S
Ho1 Ho 0.00084(6) 0.0000 0.33326(6) 0.0110(2) Uani 1 2 d S
Ho2 Ho 0.17599(6) 0.0000 0.53257(7) 0.0130(2) Uani 1 2 d S
Ho3 Ho 0.19070(6) 0.0000 0.31877(7) 0.0125(2) Uani 1 2 d S
Ho4 Ho 0.33751(6) 0.0000 0.02033(7) 0.0127(2) Uani 1 2 d S
Ho5 Ho 0.57403(6) 0.0000 0.17184(7) 0.0130(2) Uani 1 2 d S
Ho6 Ho 0.78129(6) 0.0000 0.19476(6) 0.0115(2) Uani 1 2 d S
Ho7 Ho 0.0000 0.5000 0.5000 0.0119(3) Uani 1 4 d S
Ho8 Ho 0.0000 0.0000 0.0000 0.0119(3) Uani 1 4 d S
Te1 Te 0.36639(8) 0.0000 0.33737(9) 0.0101(3) Uani 1 2 d S
Te2 Te 0.06506(8) 0.0000 0.85018(9) 0.0106(3) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ho Ho -0.2175 4.6783 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Au Au -2.0133 8.8022 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Ho6 Au1 Ho6 86.55(4) 3_455 3_445
Ho6 Au1 Ho4 136.77(4) 3_455 7_545
Ho6 Au1 Ho4 78.82(3) 3_445 7_545
Ho6 Au1 Ho4 78.82(3) 3_455 7
Ho6 Au1 Ho4 136.77(4) 3_445 7
Ho4 Au1 Ho4 84.57(4) 7_545 7
Ho6 Au1 Ho5 132.23(4) 3_455 3_445
Ho6 Au1 Ho5 75.98(3) 3_445 3_445
Ho4 Au1 Ho5 83.24(3) 7_545 3_445
Ho4 Au1 Ho5 141.24(4) 7 3_445
Ho6 Au1 Ho5 75.98(3) 3_455 3_455
Ho6 Au1 Ho5 132.23(4) 3_445 3_455
Ho4 Au1 Ho5 141.24(4) 7_545 3_455
Ho4 Au1 Ho5 83.24(3) 7 3_455
Ho5 Au1 Ho5 83.67(4) 3_445 3_455
Ho6 Au1 Ho8 136.480(19) 3_455 .
Ho6 Au1 Ho8 136.480(19) 3_445 .
Ho4 Au1 Ho8 72.04(3) 7_545 .
Ho4 Au1 Ho8 72.04(3) 7 .
Ho5 Au1 Ho8 69.20(3) 3_445 .
Ho5 Au1 Ho8 69.20(3) 3_455 .
Ho6 Au1 Ho3 67.69(3) 3_455 .
Ho6 Au1 Ho3 67.69(3) 3_445 .
Ho4 Au1 Ho3 137.688(19) 7_545 .
Ho4 Au1 Ho3 137.688(19) 7 .
Ho5 Au1 Ho3 64.53(3) 3_445 .
Ho5 Au1 Ho3 64.53(3) 3_455 .
Ho8 Au1 Ho3 116.29(3) . .
Ho3 Au2 Ho3 87.35(4) 7_556 7_546
Ho3 Au2 Ho1 73.27(3) 7_556 7_556
Ho3 Au2 Ho1 130.92(5) 7_546 7_556
Ho3 Au2 Ho1 130.92(5) 7_556 7_546
Ho3 Au2 Ho1 73.27(3) 7_546 7_546
Ho1 Au2 Ho1 86.10(4) 7_556 7_546
Ho3 Au2 Ho2 135.14(4) 7_556 7_546
Ho3 Au2 Ho2 77.76(3) 7_546 7_546
Ho1 Au2 Ho2 145.21(4) 7_556 7_546
Ho1 Au2 Ho2 84.89(3) 7_546 7_546
Ho3 Au2 Ho2 77.76(3) 7_556 7_556
Ho3 Au2 Ho2 135.14(4) 7_546 7_556
Ho1 Au2 Ho2 84.89(3) 7_556 7_556
Ho1 Au2 Ho2 145.21(4) 7_546 7_556
Ho2 Au2 Ho2 83.63(4) 7_546 7_556
Ho3 Au2 Ho7 135.954(19) 7_556 3_545
Ho3 Au2 Ho7 135.954(19) 7_546 3_545
Ho1 Au2 Ho7 70.83(3) 7_556 3_545
Ho1 Au2 Ho7 70.83(3) 7_546 3_545
Ho2 Au2 Ho7 74.47(3) 7_546 3_545
Ho2 Au2 Ho7 74.47(3) 7_556 3_545
Ho3 Au2 Ho2 67.12(3) 7_556 .
Ho3 Au2 Ho2 67.12(3) 7_546 .
Ho1 Au2 Ho2 135.58(2) 7_556 .
Ho1 Au2 Ho2 135.58(2) 7_546 .
Ho2 Au2 Ho2 68.10(3) 7_546 .
Ho2 Au2 Ho2 68.10(3) 7_556 .
Ho7 Au2 Ho2 128.91(4) 3_545 .
Au2 Ho1 Au2 86.10(4) 7_556 7_546
Au2 Ho1 Te2 116.85(4) 7_556 5_556
Au2 Ho1 Te2 116.85(4) 7_546 5_556
Au2 Ho1 Te1 155.77(5) 7_556 3_445
Au2 Ho1 Te1 92.55(3) 7_546 3_445
Te2 Ho1 Te1 85.29(4) 5_556 3_445
Au2 Ho1 Te1 92.55(3) 7_556 3_455
Au2 Ho1 Te1 155.77(5) 7_546 3_455
Te2 Ho1 Te1 85.29(4) 5_556 3_455
Te1 Ho1 Te1 78.89(4) 3_445 3_455
Au2 Ho1 Ho7 56.23(2) 7_556 .
Au2 Ho1 Ho7 103.39(4) 7_546 .
Te2 Ho1 Ho7 139.04(2) 5_556 .
Te1 Ho1 Ho7 100.91(4) 3_445 .
Te1 Ho1 Ho7 57.07(3) 3_455 .
Au2 Ho1 Ho7 103.39(4) 7_556 1_545
Au2 Ho1 Ho7 56.23(2) 7_546 1_545
Te2 Ho1 Ho7 139.04(2) 5_556 1_545
Te1 Ho1 Ho7 57.07(3) 3_445 1_545
Te1 Ho1 Ho7 100.91(4) 3_455 1_545
Ho7 Ho1 Ho7 70.45(2) . 1_545
Au2 Ho1 Ho3 52.92(2) 7_556 .
Au2 Ho1 Ho3 52.92(2) 7_546 .
Te2 Ho1 Ho3 93.77(4) 5_556 .
Te1 Ho1 Ho3 140.50(2) 3_445 .
Te1 Ho1 Ho3 140.50(2) 3_455 .
Ho7 Ho1 Ho3 105.14(3) . .
Ho7 Ho1 Ho3 105.14(3) 1_545 .
Au2 Ho1 Ho5 106.36(4) 7_556 3_445
Au2 Ho1 Ho5 64.98(3) 7_546 3_445
Te2 Ho1 Ho5 52.46(3) 5_556 3_445
Te1 Ho1 Ho5 94.84(3) 3_445 3_445
Te1 Ho1 Ho5 137.74(4) 3_455 3_445
Ho7 Ho1 Ho5 160.97(3) . 3_445
Ho7 Ho1 Ho5 110.486(16) 1_545 3_445
Ho3 Ho1 Ho5 55.90(2) . 3_445
Au2 Ho1 Ho5 64.98(3) 7_556 3_455
Au2 Ho1 Ho5 106.36(4) 7_546 3_455
Te2 Ho1 Ho5 52.46(3) 5_556 3_455
Te1 Ho1 Ho5 137.74(4) 3_445 3_455
Te1 Ho1 Ho5 94.84(3) 3_455 3_455
Ho7 Ho1 Ho5 110.486(16) . 3_455
Ho7 Ho1 Ho5 160.97(3) 1_545 3_455
Ho3 Ho1 Ho5 55.90(2) . 3_455
Ho5 Ho1 Ho5 62.14(2) 3_445 3_455
Au2 Ho2 Au2 83.63(4) 7_546 7_556
Au2 Ho2 Te1 147.14(5) 7_546 7_556
Au2 Ho2 Te1 90.48(3) 7_556 7_556
Au2 Ho2 Te1 90.48(3) 7_546 7_546
Au2 Ho2 Te1 147.14(5) 7_556 7_546
Te1 Ho2 Te1 77.17(4) 7_556 7_546
Au2 Ho2 Au2 111.90(3) 7_546 .
Au2 Ho2 Au2 111.90(3) 7_556 .
Te1 Ho2 Au2 100.31(4) 7_556 .
Te1 Ho2 Au2 100.31(4) 7_546 .
Au2 Ho2 Ho3 159.34(4) 7_546 7_556
Au2 Ho2 Ho3 101.43(2) 7_556 7_556
Te1 Ho2 Ho3 53.43(3) 7_556 7_556
Te1 Ho2 Ho3 95.40(4) 7_546 7_556
Au2 Ho2 Ho3 47.55(2) . 7_556
Au2 Ho2 Ho3 101.43(2) 7_546 7_546
Au2 Ho2 Ho3 159.34(4) 7_556 7_546
Te1 Ho2 Ho3 95.40(4) 7_556 7_546
Te1 Ho2 Ho3 53.43(3) 7_546 7_546
Au2 Ho2 Ho3 47.55(2) . 7_546
Ho3 Ho2 Ho3 67.15(3) 7_556 7_546
Au2 Ho2 Ho7 53.41(2) 7_546 1_545
Au2 Ho2 Ho7 97.60(3) 7_556 1_545
Te1 Ho2 Ho7 95.79(3) 7_556 1_545
Te1 Ho2 Ho7 54.53(3) 7_546 1_545
Au2 Ho2 Ho7 146.002(13) . 1_545
Ho3 Ho2 Ho7 143.42(4) 7_556 1_545
Ho3 Ho2 Ho7 101.48(2) 7_546 1_545
Au2 Ho2 Ho7 97.60(3) 7_546 .
Au2 Ho2 Ho7 53.41(2) 7_556 .
Te1 Ho2 Ho7 54.53(3) 7_556 .
Te1 Ho2 Ho7 95.79(3) 7_546 .
Au2 Ho2 Ho7 146.002(13) . .
Ho3 Ho2 Ho7 101.48(2) 7_556 .
Ho3 Ho2 Ho7 143.42(4) 7_546 .
Ho7 Ho2 Ho7 66.21(2) 1_545 .
Au2 Ho2 Ho3 49.87(2) 7_546 .
Au2 Ho2 Ho3 49.87(2) 7_556 .
Te1 Ho2 Ho3 139.58(2) 7_556 .
Te1 Ho2 Ho3 139.58(2) 7_546 .
Au2 Ho2 Ho3 89.89(3) . .
Ho3 Ho2 Ho3 119.15(3) 7_556 .
Ho3 Ho2 Ho3 119.15(3) 7_546 .
Ho7 Ho2 Ho3 96.98(3) 1_545 .
Ho7 Ho2 Ho3 96.98(3) . .
Au2 Ho2 Ho2 105.62(4) 7_546 7_556
Au2 Ho2 Ho2 63.24(3) 7_556 7_556
Te1 Ho2 Ho2 100.31(3) 7_556 7_556
Te1 Ho2 Ho2 148.44(6) 7_546 7_556
Au2 Ho2 Ho2 48.67(3) . 7_556
Ho3 Ho2 Ho2 60.72(3) 7_556 7_556
Ho3 Ho2 Ho2 96.18(4) 7_546 7_556
Ho7 Ho2 Ho2 154.80(5) 1_545 7_556
Ho7 Ho2 Ho2 108.39(2) . 7_556
Ho3 Ho2 Ho2 58.44(3) . 7_556
Au2 Ho2 Ho2 63.24(3) 7_546 7_546
Au2 Ho2 Ho2 105.62(4) 7_556 7_546
Te1 Ho2 Ho2 148.44(6) 7_556 7_546
Te1 Ho2 Ho2 100.31(3) 7_546 7_546
Au2 Ho2 Ho2 48.67(3) . 7_546
Ho3 Ho2 Ho2 96.18(4) 7_556 7_546
Ho3 Ho2 Ho2 60.72(3) 7_546 7_546
Ho7 Ho2 Ho2 108.39(2) 1_545 7_546
Ho7 Ho2 Ho2 154.80(5) . 7_546
Ho3 Ho2 Ho2 58.44(3) . 7_546
Ho2 Ho2 Ho2 65.31(3) 7_556 7_546
Au2 Ho3 Au2 87.35(4) 7_556 7_546
Au2 Ho3 Te1 120.83(3) 7_556 .
Au2 Ho3 Te1 120.83(3) 7_546 .
Au2 Ho3 Au1 122.51(3) 7_556 .
Au2 Ho3 Au1 122.51(3) 7_546 .
Te1 Ho3 Au1 86.87(4) . .
Au2 Ho3 Ho5 118.62(4) 7_556 3_445
Au2 Ho3 Ho5 71.43(3) 7_546 3_445
Te1 Ho3 Ho5 119.47(4) . 3_445
Au1 Ho3 Ho5 51.41(2) . 3_445
Au2 Ho3 Ho5 71.43(3) 7_556 3_455
Au2 Ho3 Ho5 118.62(4) 7_546 3_455
Te1 Ho3 Ho5 119.47(4) . 3_455
Au1 Ho3 Ho5 51.41(2) . 3_455
Ho5 Ho3 Ho5 70.54(3) 3_445 3_455
Au2 Ho3 Ho1 53.81(2) 7_556 .
Au2 Ho3 Ho1 53.81(2) 7_546 .
Te1 Ho3 Ho1 170.40(5) . .
Au1 Ho3 Ho1 102.73(4) . .
Ho5 Ho3 Ho1 67.89(3) 3_445 .
Ho5 Ho3 Ho1 67.89(3) 3_455 .
Au2 Ho3 Ho6 169.80(3) 7_556 3_445
Au2 Ho3 Ho6 102.200(19) 7_546 3_445
Te1 Ho3 Ho6 57.17(3) . 3_445
Au1 Ho3 Ho6 49.05(2) . 3_445
Ho5 Ho3 Ho6 62.31(3) 3_445 3_445
Ho5 Ho3 Ho6 100.46(4) 3_455 3_445
Ho1 Ho3 Ho6 129.73(3) . 3_445
Au2 Ho3 Ho6 102.200(19) 7_556 3_455
Au2 Ho3 Ho6 169.80(3) 7_546 3_455
Te1 Ho3 Ho6 57.17(3) . 3_455
Au1 Ho3 Ho6 49.05(2) . 3_455
Ho5 Ho3 Ho6 100.46(4) 3_445 3_455
Ho5 Ho3 Ho6 62.31(3) 3_455 3_455
Ho1 Ho3 Ho6 129.73(3) . 3_455
Ho6 Ho3 Ho6 68.06(3) 3_445 3_455
Au2 Ho3 Ho2 65.34(3) 7_556 7_556
Au2 Ho3 Ho2 110.28(4) 7_546 7_556
Te1 Ho3 Ho2 56.49(3) . 7_556
Au1 Ho3 Ho2 126.36(3) . 7_556
Ho5 Ho3 Ho2 175.96(4) 3_445 7_556
Ho5 Ho3 Ho2 111.028(18) 3_455 7_556
Ho1 Ho3 Ho2 116.13(3) . 7_556
Ho6 Ho3 Ho2 113.65(4) 3_445 7_556
Ho6 Ho3 Ho2 77.42(3) 3_455 7_556
Au2 Ho3 Ho2 110.28(4) 7_556 7_546
Au2 Ho3 Ho2 65.34(3) 7_546 7_546
Te1 Ho3 Ho2 56.49(3) . 7_546
Au1 Ho3 Ho2 126.36(3) . 7_546
Ho5 Ho3 Ho2 111.028(18) 3_445 7_546
Ho5 Ho3 Ho2 175.96(4) 3_455 7_546
Ho1 Ho3 Ho2 116.13(3) . 7_546
Ho6 Ho3 Ho2 77.42(3) 3_445 7_546
Ho6 Ho3 Ho2 113.65(4) 3_455 7_546
Ho2 Ho3 Ho2 67.15(3) 7_556 7_546
Au2 Ho3 Ho2 52.37(2) 7_556 .
Au2 Ho3 Ho2 52.37(2) 7_546 .
Te1 Ho3 Ho2 102.71(4) . .
Au1 Ho3 Ho2 170.41(4) . .
Ho5 Ho3 Ho2 121.82(3) 3_445 .
Ho5 Ho3 Ho2 121.82(3) 3_455 .
Ho1 Ho3 Ho2 67.69(3) . .
Ho6 Ho3 Ho2 136.95(3) 3_445 .
Ho6 Ho3 Ho2 136.95(3) 3_455 .
Ho2 Ho3 Ho2 60.85(3) 7_556 .
Ho2 Ho3 Ho2 60.85(3) 7_546 .
Au1 Ho4 Au1 84.57(4) 7_545 7
Au1 Ho4 Te2 149.92(5) 7_545 7_556
Au1 Ho4 Te2 90.74(3) 7 7_556
Au1 Ho4 Te2 90.74(3) 7_545 7_546
Au1 Ho4 Te2 149.92(5) 7 7_546
Te2 Ho4 Te2 78.61(4) 7_556 7_546
Au1 Ho4 Ho8 101.13(3) 7_545 3
Au1 Ho4 Ho8 56.64(2) 7 3
Te2 Ho4 Ho8 52.93(3) 7_556 3
Te2 Ho4 Ho8 95.54(3) 7_546 3
Au1 Ho4 Ho8 56.64(2) 7_545 3_545
Au1 Ho4 Ho8 101.13(3) 7 3_545
Te2 Ho4 Ho8 95.54(3) 7_556 3_545
Te2 Ho4 Ho8 52.93(3) 7_546 3_545
Ho8 Ho4 Ho8 67.02(2) 3 3_545
Au1 Ho4 Ho4 66.83(3) 7_545 7_545
Au1 Ho4 Ho4 110.21(5) 7 7_545
Te2 Ho4 Ho4 141.42(5) 7_556 7_545
Te2 Ho4 Ho4 94.93(3) 7_546 7_545
Ho8 Ho4 Ho4 164.13(5) 3 7_545
Ho8 Ho4 Ho4 110.821(17) 3_545 7_545
Au1 Ho4 Ho4 110.21(5) 7_545 7
Au1 Ho4 Ho4 66.83(3) 7 7
Te2 Ho4 Ho4 94.93(3) 7_556 7
Te2 Ho4 Ho4 141.42(5) 7_546 7
Ho8 Ho4 Ho4 110.821(17) 3 7
Ho8 Ho4 Ho4 164.13(5) 3_545 7
Ho4 Ho4 Ho4 66.63(4) 7_545 7
Au1 Ho4 Ho6 49.94(2) 7_545 5_655
Au1 Ho4 Ho6 49.94(2) 7 5_655
Te2 Ho4 Ho6 139.57(2) 7_556 5_655
Te2 Ho4 Ho6 139.57(2) 7_546 5_655
Ho8 Ho4 Ho6 100.59(3) 3 5_655
Ho8 Ho4 Ho6 100.59(3) 3_545 5_655
Ho4 Ho4 Ho6 63.90(3) 7_545 5_655
Ho4 Ho4 Ho6 63.90(3) 7 5_655
Au1 Ho4 Ho6 159.74(4) 7_545 3_455
Au1 Ho4 Ho6 104.43(2) 7 3_455
Te2 Ho4 Ho6 49.57(3) 7_556 3_455
Te2 Ho4 Ho6 90.00(4) 7_546 3_455
Ho8 Ho4 Ho6 98.940(19) 3 3_455
Ho8 Ho4 Ho6 136.11(3) 3_545 3_455
Ho4 Ho4 Ho6 92.95(4) 7_545 3_455
Ho4 Ho4 Ho6 59.27(3) 7 3_455
Ho6 Ho4 Ho6 123.17(3) 5_655 3_455
Au1 Ho4 Ho6 104.43(2) 7_545 3_445
Au1 Ho4 Ho6 159.74(4) 7 3_445
Te2 Ho4 Ho6 90.00(4) 7_556 3_445
Te2 Ho4 Ho6 49.57(3) 7_546 3_445
Ho8 Ho4 Ho6 136.11(3) 3 3_445
Ho8 Ho4 Ho6 98.940(19) 3_545 3_445
Ho4 Ho4 Ho6 59.27(3) 7_545 3_445
Ho4 Ho4 Ho6 92.95(4) 7 3_445
Ho6 Ho4 Ho6 123.17(3) 5_655 3_445
Ho6 Ho4 Ho6 61.58(2) 3_455 3_445
Au1 Ho4 Ho5 48.66(2) 7_545 5_655
Au1 Ho4 Ho5 48.66(2) 7 5_655
Te2 Ho4 Ho5 107.83(4) 7_556 5_655
Te2 Ho4 Ho5 107.83(4) 7_546 5_655
Ho8 Ho4 Ho5 54.911(18) 3 5_655
Ho8 Ho4 Ho5 54.911(18) 3_545 5_655
Ho4 Ho4 Ho5 110.32(4) 7_545 5_655
Ho4 Ho4 Ho5 110.32(4) 7 5_655
Ho6 Ho4 Ho5 56.32(3) 5_655 5_655
Ho6 Ho4 Ho5 148.705(13) 3_455 5_655
Ho6 Ho4 Ho5 148.705(13) 3_445 5_655
Au1 Ho5 Au1 83.67(4) 3 3_545
Au1 Ho5 Te2 153.52(5) 3 7_546
Au1 Ho5 Te2 92.72(3) 3_545 7_546
Au1 Ho5 Te2 92.72(3) 3 7_556
Au1 Ho5 Te2 153.52(5) 3_545 7_556
Te2 Ho5 Te2 78.91(4) 7_546 7_556
Au1 Ho5 Ho3 64.06(3) 3 3
Au1 Ho5 Ho3 109.43(4) 3_545 3
Te2 Ho5 Ho3 140.51(5) 7_546 3
Te2 Ho5 Ho3 92.17(3) 7_556 3
Au1 Ho5 Ho3 109.43(4) 3 3_545
Au1 Ho5 Ho3 64.06(3) 3_545 3_545
Te2 Ho5 Ho3 92.17(3) 7_546 3_545
Te2 Ho5 Ho3 140.51(5) 7_556 3_545
Ho3 Ho5 Ho3 70.54(3) 3 3_545
Au1 Ho5 Ho8 103.15(4) 3 3_545
Au1 Ho5 Ho8 57.85(2) 3_545 3_545
Te2 Ho5 Ho8 54.18(3) 7_546 3_545
Te2 Ho5 Ho8 97.96(4) 7_556 3_545
Ho3 Ho5 Ho8 164.17(4) 3 3_545
Ho3 Ho5 Ho8 107.723(16) 3_545 3_545
Au1 Ho5 Ho8 57.85(2) 3 3
Au1 Ho5 Ho8 103.15(4) 3_545 3
Te2 Ho5 Ho8 97.96(4) 7_546 3
Te2 Ho5 Ho8 54.18(3) 7_556 3
Ho3 Ho5 Ho8 107.723(16) 3 3
Ho3 Ho5 Ho8 164.17(4) 3_545 3
Ho8 Ho5 Ho8 69.43(2) 3_545 3
Au1 Ho5 Ho6 51.01(2) 3 .
Au1 Ho5 Ho6 51.01(2) 3_545 .
Te2 Ho5 Ho6 140.47(2) 7_546 .
Te2 Ho5 Ho6 140.47(2) 7_556 .
Ho3 Ho5 Ho6 60.33(3) 3 .
Ho3 Ho5 Ho6 60.33(3) 3_545 .
Ho8 Ho5 Ho6 104.70(3) 3_545 .
Ho8 Ho5 Ho6 104.70(3) 3 .
Au1 Ho5 Ho1 103.09(2) 3 3
Au1 Ho5 Ho1 156.19(4) 3_545 3
Te2 Ho5 Ho1 90.77(3) 7_546 3
Te2 Ho5 Ho1 50.02(3) 7_556 3
Ho3 Ho5 Ho1 56.22(3) 3 3
Ho3 Ho5 Ho1 92.29(3) 3_545 3
Ho8 Ho5 Ho1 139.10(3) 3_545 3
Ho8 Ho5 Ho1 99.67(2) 3 3
Ho6 Ho5 Ho1 116.20(3) . 3
Au1 Ho5 Ho1 156.19(4) 3 3_545
Au1 Ho5 Ho1 103.09(2) 3_545 3_545
Te2 Ho5 Ho1 50.02(3) 7_546 3_545
Te2 Ho5 Ho1 90.77(3) 7_556 3_545
Ho3 Ho5 Ho1 92.29(3) 3 3_545
Ho3 Ho5 Ho1 56.22(3) 3_545 3_545
Ho8 Ho5 Ho1 99.67(2) 3_545 3_545
Ho8 Ho5 Ho1 139.10(3) 3 3_545
Ho6 Ho5 Ho1 116.20(3) . 3_545
Ho1 Ho5 Ho1 62.14(2) 3 3_545
Au1 Ho5 Ho4 48.10(2) 3 5_655
Au1 Ho5 Ho4 48.10(2) 3_545 5_655
Te2 Ho5 Ho4 111.74(4) 7_546 5_655
Te2 Ho5 Ho4 111.74(4) 7_556 5_655
Ho3 Ho5 Ho4 107.32(3) 3 5_655
Ho3 Ho5 Ho4 107.32(3) 3_545 5_655
Ho8 Ho5 Ho4 57.57(2) 3_545 5_655
Ho8 Ho5 Ho4 57.57(2) 3 5_655
Ho6 Ho5 Ho4 58.70(3) . 5_655
Ho1 Ho5 Ho4 148.928(12) 3 5_655
Ho1 Ho5 Ho4 148.928(12) 3_545 5_655
Au1 Ho6 Au1 86.55(4) 3_545 3
Au1 Ho6 Te2 115.15(4) 3_545 5_656
Au1 Ho6 Te2 115.15(4) 3 5_656
Au1 Ho6 Te1 158.21(5) 3_545 3
Au1 Ho6 Te1 94.36(3) 3 3
Te2 Ho6 Te1 84.16(4) 5_656 3
Au1 Ho6 Te1 94.36(3) 3_545 3_545
Au1 Ho6 Te1 158.21(5) 3 3_545
Te2 Ho6 Te1 84.16(4) 5_656 3_545
Te1 Ho6 Te1 76.90(4) 3 3_545
Au1 Ho6 Ho3 108.50(4) 3_545 3
Au1 Ho6 Ho3 63.26(3) 3 3
Te2 Ho6 Ho3 136.22(3) 5_656 3
Te1 Ho6 Ho3 53.81(3) 3 3
Te1 Ho6 Ho3 96.06(4) 3_545 3
Au1 Ho6 Ho3 63.26(3) 3_545 3_545
Au1 Ho6 Ho3 108.50(4) 3 3_545
Te2 Ho6 Ho3 136.22(3) 5_656 3_545
Te1 Ho6 Ho3 96.06(4) 3 3_545
Te1 Ho6 Ho3 53.81(3) 3_545 3_545
Ho3 Ho6 Ho3 68.06(3) 3 3_545
Au1 Ho6 Ho5 53.02(2) 3_545 .
Au1 Ho6 Ho5 53.02(2) 3 .
Te2 Ho6 Ho5 160.00(5) 5_656 .
Te1 Ho6 Ho5 111.17(4) 3 .
Te1 Ho6 Ho5 111.17(4) 3_545 .
Ho3 Ho6 Ho5 57.36(2) 3 .
Ho3 Ho6 Ho5 57.36(2) 3_545 .
Au1 Ho6 Ho4 51.24(2) 3_545 5_655
Au1 Ho6 Ho4 51.24(2) 3 5_655
Te2 Ho6 Ho4 95.02(4) 5_656 5_655
Te1 Ho6 Ho4 141.48(2) 3 5_655
Te1 Ho6 Ho4 141.48(2) 3_545 5_655
Ho3 Ho6 Ho4 110.01(3) 3 5_655
Ho3 Ho6 Ho4 110.01(3) 3_545 5_655
Ho5 Ho6 Ho4 64.98(3) . 5_655
Au1 Ho6 Ho4 63.43(3) 3_545 3_545
Au1 Ho6 Ho4 104.74(4) 3 3_545
Te2 Ho6 Ho4 52.28(3) 5_656 3_545
Te1 Ho6 Ho4 136.41(4) 3 3_545
Te1 Ho6 Ho4 95.03(3) 3_545 3_545
Ho3 Ho6 Ho4 166.79(4) 3 3_545
Ho3 Ho6 Ho4 113.616(17) 3_545 3_545
Ho5 Ho6 Ho4 111.63(3) . 3_545
Ho4 Ho6 Ho4 56.83(3) 5_655 3_545
Au1 Ho6 Ho4 104.74(4) 3_545 3
Au1 Ho6 Ho4 63.43(3) 3 3
Te2 Ho6 Ho4 52.28(3) 5_656 3
Te1 Ho6 Ho4 95.03(3) 3 3
Te1 Ho6 Ho4 136.41(4) 3_545 3
Ho3 Ho6 Ho4 113.616(17) 3 3
Ho3 Ho6 Ho4 166.79(4) 3_545 3
Ho5 Ho6 Ho4 111.63(3) . 3
Ho4 Ho6 Ho4 56.83(3) 5_655 3
Ho4 Ho6 Ho4 61.58(2) 3_545 3
Au2 Ho7 Au2 180.0 7_556 3_455
Au2 Ho7 Te1 90.19(3) 7_556 7_556
Au2 Ho7 Te1 89.81(3) 3_455 7_556
Au2 Ho7 Te1 89.81(3) 7_556 3_455
Au2 Ho7 Te1 90.19(3) 3_455 3_455
Te1 Ho7 Te1 180.0 7_556 3_455
Au2 Ho7 Ho1 52.94(2) 7_556 .
Au2 Ho7 Ho1 127.06(2) 3_455 .
Te1 Ho7 Ho1 123.61(2) 7_556 .
Te1 Ho7 Ho1 56.39(2) 3_455 .
Au2 Ho7 Ho1 127.06(2) 7_556 5_566
Au2 Ho7 Ho1 52.94(2) 3_455 5_566
Te1 Ho7 Ho1 56.39(2) 7_556 5_566
Te1 Ho7 Ho1 123.61(2) 3_455 5_566
Ho1 Ho7 Ho1 180.0 . 5_566
Au2 Ho7 Ho1 52.94(2) 7_556 1_565
Au2 Ho7 Ho1 127.06(2) 3_455 1_565
Te1 Ho7 Ho1 123.61(2) 7_556 1_565
Te1 Ho7 Ho1 56.39(2) 3_455 1_565
Ho1 Ho7 Ho1 70.45(2) . 1_565
Ho1 Ho7 Ho1 109.55(2) 5_566 1_565
Au2 Ho7 Ho1 127.06(2) 7_556 5_556
Au2 Ho7 Ho1 52.94(2) 3_455 5_556
Te1 Ho7 Ho1 56.39(2) 7_556 5_556
Te1 Ho7 Ho1 123.61(2) 3_455 5_556
Ho1 Ho7 Ho1 109.55(2) . 5_556
Ho1 Ho7 Ho1 70.45(2) 5_566 5_556
Ho1 Ho7 Ho1 180.0 1_565 5_556
Au2 Ho7 Ho2 52.12(2) 7_556 1_565
Au2 Ho7 Ho2 127.88(2) 3_455 1_565
Te1 Ho7 Ho2 55.41(3) 7_556 1_565
Te1 Ho7 Ho2 124.59(3) 3_455 1_565
Ho1 Ho7 Ho2 105.02(2) . 1_565
Ho1 Ho7 Ho2 74.98(2) 5_566 1_565
Ho1 Ho7 Ho2 68.24(2) 1_565 1_565
Ho1 Ho7 Ho2 111.76(2) 5_556 1_565
Au2 Ho7 Ho2 127.88(2) 7_556 5_556
Au2 Ho7 Ho2 52.12(2) 3_455 5_556
Te1 Ho7 Ho2 124.59(3) 7_556 5_556
Te1 Ho7 Ho2 55.41(3) 3_455 5_556
Ho1 Ho7 Ho2 74.98(2) . 5_556
Ho1 Ho7 Ho2 105.02(2) 5_566 5_556
Ho1 Ho7 Ho2 111.76(2) 1_565 5_556
Ho1 Ho7 Ho2 68.24(2) 5_556 5_556
Ho2 Ho7 Ho2 180.00(4) 1_565 5_556
Au2 Ho7 Ho2 52.12(2) 7_556 .
Au2 Ho7 Ho2 127.88(2) 3_455 .
Te1 Ho7 Ho2 55.41(2) 7_556 .
Te1 Ho7 Ho2 124.59(2) 3_455 .
Ho1 Ho7 Ho2 68.24(2) . .
Ho1 Ho7 Ho2 111.76(2) 5_566 .
Ho1 Ho7 Ho2 105.02(2) 1_565 .
Ho1 Ho7 Ho2 74.98(2) 5_556 .
Ho2 Ho7 Ho2 66.21(2) 1_565 .
Ho2 Ho7 Ho2 113.79(2) 5_556 .
Au2 Ho7 Ho2 127.88(2) 7_556 5_566
Au2 Ho7 Ho2 52.12(2) 3_455 5_566
Te1 Ho7 Ho2 124.59(3) 7_556 5_566
Te1 Ho7 Ho2 55.41(2) 3_455 5_566
Ho1 Ho7 Ho2 111.76(2) . 5_566
Ho1 Ho7 Ho2 68.24(2) 5_566 5_566
Ho1 Ho7 Ho2 74.98(2) 1_565 5_566
Ho1 Ho7 Ho2 105.02(2) 5_556 5_566
Ho2 Ho7 Ho2 113.79(2) 1_565 5_566
Ho2 Ho7 Ho2 66.21(2) 5_556 5_566
Ho2 Ho7 Ho2 180.00(4) . 5_566
Te2 Ho8 Te2 180.00(4) 5_556 1_554
Te2 Ho8 Au1 88.90(3) 5_556 5
Te2 Ho8 Au1 91.10(3) 1_554 5
Te2 Ho8 Au1 91.10(3) 5_556 .
Te2 Ho8 Au1 88.90(3) 1_554 .
Au1 Ho8 Au1 180.00(4) 5 .
Te2 Ho8 Ho5 123.20(3) 5_556 7_545
Te2 Ho8 Ho5 56.80(3) 1_554 7_545
Au1 Ho8 Ho5 52.956(19) 5 7_545
Au1 Ho8 Ho5 127.044(19) . 7_545
Te2 Ho8 Ho5 56.80(3) 5_556 3_455
Te2 Ho8 Ho5 123.20(3) 1_554 3_455
Au1 Ho8 Ho5 127.044(19) 5 3_455
Au1 Ho8 Ho5 52.956(19) . 3_455
Ho5 Ho8 Ho5 180.00(3) 7_545 3_455
Te2 Ho8 Ho5 123.20(3) 5_556 7
Te2 Ho8 Ho5 56.80(3) 1_554 7
Au1 Ho8 Ho5 52.956(19) 5 7
Au1 Ho8 Ho5 127.044(19) . 7
Ho5 Ho8 Ho5 69.43(2) 7_545 7
Ho5 Ho8 Ho5 110.57(2) 3_455 7
Te2 Ho8 Ho5 56.80(3) 5_556 3_445
Te2 Ho8 Ho5 123.20(3) 1_554 3_445
Au1 Ho8 Ho5 127.044(19) 5 3_445
Au1 Ho8 Ho5 52.956(19) . 3_445
Ho5 Ho8 Ho5 110.57(2) 7_545 3_445
Ho5 Ho8 Ho5 69.43(2) 3_455 3_445
Ho5 Ho8 Ho5 180.00(5) 7 3_445
Te2 Ho8 Ho4 55.69(3) 5_556 3_445
Te2 Ho8 Ho4 124.31(3) 1_554 3_445
Au1 Ho8 Ho4 51.31(2) 5 3_445
Au1 Ho8 Ho4 128.69(2) . 3_445
Ho5 Ho8 Ho4 67.52(2) 7_545 3_445
Ho5 Ho8 Ho4 112.48(2) 3_455 3_445
Ho5 Ho8 Ho4 104.27(2) 7 3_445
Ho5 Ho8 Ho4 75.73(2) 3_445 3_445
Te2 Ho8 Ho4 124.31(3) 5_556 7
Te2 Ho8 Ho4 55.69(3) 1_554 7
Au1 Ho8 Ho4 128.69(2) 5 7
Au1 Ho8 Ho4 51.31(2) . 7
Ho5 Ho8 Ho4 112.48(2) 7_545 7
Ho5 Ho8 Ho4 67.52(2) 3_455 7
Ho5 Ho8 Ho4 75.73(2) 7 7
Ho5 Ho8 Ho4 104.27(2) 3_445 7
Ho4 Ho8 Ho4 180.00(3) 3_445 7
Te2 Ho8 Ho4 55.69(3) 5_556 3_455
Te2 Ho8 Ho4 124.31(3) 1_554 3_455
Au1 Ho8 Ho4 51.31(2) 5 3_455
Au1 Ho8 Ho4 128.69(2) . 3_455
Ho5 Ho8 Ho4 104.27(2) 7_545 3_455
Ho5 Ho8 Ho4 75.73(2) 3_455 3_455
Ho5 Ho8 Ho4 67.52(2) 7 3_455
Ho5 Ho8 Ho4 112.48(2) 3_445 3_455
Ho4 Ho8 Ho4 67.02(2) 3_445 3_455
Ho4 Ho8 Ho4 112.98(2) 7 3_455
Te2 Ho8 Ho4 124.31(3) 5_556 7_545
Te2 Ho8 Ho4 55.69(3) 1_554 7_545
Au1 Ho8 Ho4 128.69(2) 5 7_545
Au1 Ho8 Ho4 51.31(2) . 7_545
Ho5 Ho8 Ho4 75.73(2) 7_545 7_545
Ho5 Ho8 Ho4 104.27(2) 3_455 7_545
Ho5 Ho8 Ho4 112.48(2) 7 7_545
Ho5 Ho8 Ho4 67.52(2) 3_445 7_545
Ho4 Ho8 Ho4 112.98(2) 3_445 7_545
Ho4 Ho8 Ho4 67.02(2) 7 7_545
Ho4 Ho8 Ho4 180.00(3) 3_455 7_545
Ho3 Te1 Ho1 140.00(2) . 3
Ho3 Te1 Ho1 140.00(2) . 3_545
Ho1 Te1 Ho1 78.89(4) 3 3_545
Ho3 Te1 Ho7 128.29(5) . 3_545
Ho1 Te1 Ho7 66.54(3) 3 3_545
Ho1 Te1 Ho7 66.54(3) 3_545 3_545
Ho3 Te1 Ho2 70.08(3) . 7_556
Ho1 Te1 Ho2 86.19(3) 3 7_556
Ho1 Te1 Ho2 136.55(6) 3_545 7_556
Ho7 Te1 Ho2 70.06(3) 3_545 7_556
Ho3 Te1 Ho2 70.08(3) . 7_546
Ho1 Te1 Ho2 136.55(6) 3 7_546
Ho1 Te1 Ho2 86.19(3) 3_545 7_546
Ho7 Te1 Ho2 70.06(3) 3_545 7_546
Ho2 Te1 Ho2 77.17(4) 7_556 7_546
Ho3 Te1 Ho6 69.02(4) . 3_445
Ho1 Te1 Ho6 126.96(5) 3 3_445
Ho1 Te1 Ho6 79.12(3) 3_545 3_445
Ho7 Te1 Ho6 140.22(2) 3_545 3_445
Ho2 Te1 Ho6 139.10(5) 7_556 3_445
Ho2 Te1 Ho6 88.87(3) 7_546 3_445
Ho3 Te1 Ho6 69.02(4) . 3_455
Ho1 Te1 Ho6 79.12(3) 3 3_455
Ho1 Te1 Ho6 126.96(5) 3_545 3_455
Ho7 Te1 Ho6 140.22(2) 3_545 3_455
Ho2 Te1 Ho6 88.87(3) 7_556 3_455
Ho2 Te1 Ho6 139.10(5) 7_546 3_455
Ho6 Te1 Ho6 76.90(4) 3_445 3_455
Ho6 Te2 Ho1 83.63(5) 5_656 5_556
Ho6 Te2 Ho8 140.26(5) 5_656 1_556
Ho1 Te2 Ho8 136.12(5) 5_556 1_556
Ho6 Te2 Ho5 135.45(3) 5_656 7_546
Ho1 Te2 Ho5 77.52(4) 5_556 7_546
Ho8 Te2 Ho5 69.02(3) 1_556 7_546
Ho6 Te2 Ho5 135.45(3) 5_656 7_556
Ho1 Te2 Ho5 77.52(4) 5_556 7_556
Ho8 Te2 Ho5 69.02(3) 1_556 7_556
Ho5 Te2 Ho5 78.91(4) 7_546 7_556
Ho6 Te2 Ho4 78.16(4) 5_656 7_556
Ho1 Te2 Ho4 135.95(3) 5_556 7_556
Ho8 Te2 Ho4 71.38(4) 1_556 7_556
Ho5 Te2 Ho4 140.39(5) 7_546 7_556
Ho5 Te2 Ho4 88.02(3) 7_556 7_556
Ho6 Te2 Ho4 78.16(4) 5_656 7_546
Ho1 Te2 Ho4 135.95(3) 5_556 7_546
Ho8 Te2 Ho4 71.38(4) 1_556 7_546
Ho5 Te2 Ho4 88.02(3) 7_546 7_546
Ho5 Te2 Ho4 140.39(6) 7_556 7_546
Ho4 Te2 Ho4 78.61(4) 7_556 7_546
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Au1 Ho6 2.9228(10) 3_455
Au1 Ho6 2.9228(10) 3_445
Au1 Ho4 2.9779(11) 7_545
Au1 Ho4 2.9779(11) 7
Au1 Ho5 3.0042(10) 3_445
Au1 Ho5 3.0042(10) 3_455
Au1 Ho8 3.1866(10) .
Au1 Ho3 3.4561(15) .
Au2 Ho3 2.9015(10) 7_556
Au2 Ho3 2.9015(10) 7_546
Au2 Ho1 2.9351(11) 7_556
Au2 Ho1 2.9351(10) 7_546
Au2 Ho2 3.0052(11) 7_546
Au2 Ho2 3.0052(11) 7_556
Au2 Ho7 3.0574(9) 3_545
Au2 Ho2 3.5736(15) .
Ho1 Au2 2.9351(10) 7_556
Ho1 Au2 2.9351(10) 7_546
Ho1 Te2 3.0470(19) 5_556
Ho1 Te1 3.1537(13) 3_445
Ho1 Te1 3.1537(13) 3_455
Ho1 Ho7 3.4739(9) .
Ho1 Ho7 3.4739(9) 1_545
Ho1 Ho3 3.4829(15) .
Ho1 Ho5 3.8823(13) 3_445
Ho1 Ho5 3.8823(13) 3_455
Ho2 Au2 3.0052(11) 7_546
Ho2 Au2 3.0052(11) 7_556
Ho2 Te1 3.2128(14) 7_556
Ho2 Te1 3.2128(14) 7_546
Ho2 Ho3 3.6228(13) 7_556
Ho2 Ho3 3.6228(13) 7_546
Ho2 Ho7 3.6687(10) 1_545
Ho2 Ho7 3.6687(10) .
Ho2 Ho3 3.7085(16) .
Ho2 Ho2 3.7134(17) 7_556
Ho2 Ho2 3.7134(17) 7_546
Ho3 Au2 2.9015(10) 7_556
Ho3 Au2 2.9015(10) 7_546
Ho3 Te1 3.0949(17) .
Ho3 Ho5 3.4701(12) 3_445
Ho3 Ho5 3.4701(12) 3_455
Ho3 Ho6 3.5805(12) 3_445
Ho3 Ho6 3.5805(12) 3_455
Ho3 Ho2 3.6228(13) 7_556
Ho3 Ho2 3.6228(13) 7_546
Ho4 Au1 2.9779(11) 7_545
Ho4 Au1 2.9779(11) 7
Ho4 Te2 3.1631(14) 7_556
Ho4 Te2 3.1631(14) 7_546
Ho4 Ho8 3.6292(9) 3
Ho4 Ho8 3.6292(9) 3_545
Ho4 Ho4 3.6481(17) 7_545
Ho4 Ho4 3.6481(17) 7
Ho4 Ho6 3.7465(16) 5_655
Ho4 Ho6 3.9139(13) 3_455
Ho4 Ho6 3.9139(13) 3_445
Ho4 Ho5 3.9732(16) 5_655
Ho5 Au1 3.0042(10) 3
Ho5 Au1 3.0042(10) 3_545
Ho5 Te2 3.1530(13) 7_546
Ho5 Te2 3.1530(13) 7_556
Ho5 Ho3 3.4701(12) 3
Ho5 Ho3 3.4701(12) 3_545
Ho5 Ho8 3.5184(10) 3_545
Ho5 Ho8 3.5184(10) 3
Ho5 Ho6 3.6486(15) .
Ho5 Ho1 3.8823(13) 3
Ho5 Ho1 3.8823(13) 3_545
Ho5 Ho4 3.9732(16) 5_655
Ho6 Au1 2.9228(10) 3_545
Ho6 Au1 2.9228(10) 3
Ho6 Te2 3.0439(17) 5_656
Ho6 Te1 3.2221(14) 3
Ho6 Te1 3.2221(14) 3_545
Ho6 Ho3 3.5805(12) 3
Ho6 Ho3 3.5805(12) 3_545
Ho6 Ho4 3.7465(16) 5_655
Ho6 Ho4 3.9139(13) 3_545
Ho6 Ho4 3.9139(13) 3
Ho7 Au2 3.0574(9) 7_556
Ho7 Au2 3.0574(9) 3_455
Ho7 Te1 3.1784(15) 7_556
Ho7 Te1 3.1784(15) 3_455
Ho7 Ho1 3.4739(9) 5_566
Ho7 Ho1 3.4739(9) 1_565
Ho7 Ho1 3.4739(9) 5_556
Ho7 Ho2 3.6687(10) 1_565
Ho7 Ho2 3.6687(10) 5_556
Ho7 Ho2 3.6687(10) 5_566
Ho8 Te2 3.0555(14) 5_556
Ho8 Te2 3.0555(14) 1_554
Ho8 Au1 3.1866(10) 5
Ho8 Ho5 3.5184(10) 7_545
Ho8 Ho5 3.5184(10) 3_455
Ho8 Ho5 3.5184(10) 7
Ho8 Ho5 3.5184(10) 3_445
Ho8 Ho4 3.6292(9) 3_445
Ho8 Ho4 3.6292(9) 7
Ho8 Ho4 3.6292(9) 3_455
Ho8 Ho4 3.6292(9) 7_545
Te1 Ho1 3.1537(13) 3
Te1 Ho1 3.1537(13) 3_545
Te1 Ho7 3.1784(15) 3_545
Te1 Ho2 3.2128(14) 7_556
Te1 Ho2 3.2128(14) 7_546
Te1 Ho6 3.2221(14) 3_445
Te1 Ho6 3.2221(14) 3_455
Te2 Ho6 3.0439(17) 5_656
Te2 Ho1 3.0470(19) 5_556
Te2 Ho8 3.0555(14) 1_556
Te2 Ho5 3.1530(13) 7_546
Te2 Ho5 3.1530(13) 7_556
Te2 Ho4 3.1631(14) 7_556
Te2 Ho4 3.1631(14) 7_546
